Modeling the electronic properties for CNT interacted with ZnO, CuO, and Co3O4

Because of the wide applications of carbon nanotubes (CNTs) and magic properties of metal oxides, Hartree–Fock quantum mechanical calculations at HF/STO-3G were applied to study the electronic properties of CNTs and their interaction with ZnO, CuO, and Co3O4. Calculations were conducted to calculate HOMO/LUMO bandgap energy ∆E, molecular electrostatic potential (MESP), and total dipole moment (TDM) for CNTs, CNT-Zn-O, CNT-Cu-O, CNT-Co-O, and CNT-O-Zn, CNT-O-Cu, CNT-O-Co following the two mechanisms of interaction as adsorbed and complex state. The calculations show that the interaction of CNTs with metal oxides increases its reactivity where MESP indicated to more distribution charges and an increase in the TDM value after the interaction of CNTs with metal oxides. Where the interaction of CNT-Co-O as adsorbed state has the highest TDM with the lowest bandgap ∆E which confirms that CNT-Co3O4 can be used in sensing devices.


Introduction
Since the discovery of CNTs by Iijima (1991), the subject takes great attention in scientific research due to it is logical electronic physical, and mechanical properties. Where, large surface area, high thermal and electrical conductivity of CNTs make them applicable in several fields of energy storage devices such as solar cells, supercapacitors, and sensors applications (Smalley 2003;Scoville et al. 1991;Habila et al. 2017;Kamas et al. 2021). There are two main types of CNTs the first is a single-wall carbon nanotube (SWCNT) which is considered as a graphene sheet rolled up to form a single cylinder in a nanoscale. While the second type is called multiwall carbon nanotubes (MWCNT) which are several multilayers of concentric tubes (Klumpp et al. 2006;Erik et al. 2017;Soylak and Unsal 2009). Synthesizing process of CNTs is achieved by different methods. The most important and well-known methods are arc discharge, laser ablation, and chemical vapor deposition (CVD) (Awasthi et al. 2005;Isaacs et al. 2010). Functionalization of CNTs enhances its physical properties and takes nanotubes to a very wide range of applications (Morsy et al. 2015;Ytreberg et al. 2017). It must be covalent or noncovalent functionalizations. Covalent functionalization causes change hybridization from SP2 to SP3 and noncovalent such as van der Waal's force i.e. adsorption of atoms or small molecules on the outer surface of CNTs (Hirsch and Vostrowsky 2005). While noncovalent interaction and functionalization are preferred because it conserves electrical properties and does not disturb π electrons decolonization (Speranza 2019). In recent years the semiconductor metal oxides have great attention due to their magical properties of high stability, chemical, physical, electronic, and high responsibility for sensor applications (Chavali and Nikolova 2019). Researchers found that the combination between CNTs and metal oxides nanoparticles improves the sensor's responsibility (Korotcenkov and Cho 2017).
Molecular modeling is useful to understand the electronic structure, chemical and physical properties of many molecules. where the computational work attaches and simplifies the communication between theoretical and experimental results. Molecular modeling is divided into two branches, the first is called molecular mechanics which predicts the structure of molecule applying the classical physics and studies the interactions that act upon nuclei. The second one is the electronic structure methods that are solving Schrodinger equations. Electronic structure methods are divided into two classes which are semi-empirical methods and Ab initio methods. Solving the Schrodinger equation, total energy and TDM can be obtained from the first derivative of the Schrodinger equation while the vibration frequency appears in Raman and IR spectroscopy in addition to other physical parameters are obtained from the second derivative (Foresman and Frisch 1996).
Recently researchers are applying molecular modeling to understand the structural properties of carbon nanomaterials (Ezzat et al. , 2020Elhaes et al. 2018). Zollo and Gala (2012) studied the structure of carbon nanomaterials with various atomizing methods of gas adsorption one of these methods is HF method, where the interaction configuration in the ground state is replaced by a linear combination state and the excited state is replaced by virtual molecular orbitals (Young 2001).
The interactions of CNTs with metal oxides and the effect of functionalization on the surface of CNTs are explained by molecular modeling where the effect of functionalization is very important for certain well applications.
The present work aimed to study CNT and CNT interacted with ZnO, CuO, and Co 3 O 4 following the two mechanisms of interaction: adsorb and complex states. The electronic properties were studied in terms of calculated TDM, HOMO-LUMO bandgap energy, and MESP at the HF/ STO-3G level of theory.

Calculations details
All calculations were carried out using Gaussian 09 program (Frisch et al. 2010) at Spectroscopy Department, National Research Centre (NRC), Cairo, Egypt. Model molecules were subjected to optimization using HF method at STO-3G basis set (Stewart 1970). Then, three physical parameters namely HOMO/LUMO molecular orbital, TDM, and MESP were calculated for all studied structures at the same level of theory.

Building the model molecules
A model molecule was designed to form the structure of CNT. This CNT is formed by rolling graphene sheet to obtain a hollow cylinder consisting of hexagonal carbon rings of 84 carbon atoms. As shown in Fig There is also another interaction mechanism that can be studied which is the complex interaction. In this case the CNT can interact with ZnO, CuO, and Co 3 O 4 as a complex interaction. Also, this interaction can be processed throughout the metal atom as shown in Fig. 3 and throughout the oxygen atom as presented in Fig. 4.

HOMO/LUMO and MESP for CNT
HOMO and LUMO are the most important orbitals in the molecule where HOMO is the highest occupied molecular orbital and LUMO is the lowest unoccupied molecular orbital.   The difference in energy between the HOMO and LUMO orbitals gives the bandgap energy where the most excitations occur. HOMO/LUMO band gap calculations are useful to study the electrical properties of the studied structures. MESP is an important parameter to describe the nucleophilic and electrophilic active sites of CNT structure and for CNT interacted with metal oxides. Generally, MESP measures the interactions of charges around the surface. Mapping MESP contours on the surface of the nanotube enable us how to activate the CNT surface by illustrating the distribution of charges on the surface of CNT by following a color mapping. The potential is high at red color then followed decrease until blue color to red > orange > yellow > greenthan bluethan blue > blue (Murray and Sen 1996;Şahin et al. 2015). Figure 5 presented the HOMO/LUMO and MESP for CNT. Firstly, the HOMO and LUMO molecular orbitals are distributed along the surface of CNT. MESP for CNT showed that only yellow color appears refers to the uniform distribution of charges inside and outside the surface of CNT ascribed no changing in the electronegativity. Therefore, it is important to study the interaction of CNT with metal oxides to manipulate its reactivity properties. There are color changes from red to blue color in the three structures toward the metal oxides position. Such colors indicated to the active sites at the surface of CNT interacted with the three metal oxides individually. The results confirm the same obtained before (Politzer et al. 1986). Therefore, mapping colors demonstrated that the adsorption of metal oxides on the surface of nanotubes manipulates the reactivity of CNT and direct functionalized CNT toward a wide range of applications.    CNT-O-metal unlike the mapping of MESP of CNT structure. The results confirm that the CNT became more reactive due to the interaction with metal oxides. Also, Fig. 9 showed that the reactivity of CNT-O-Co model molecule is higher than that of the other models as the intensity of the red color increased within the structure. Meanwhile, there are more charges transferred on the CNT surface when the interaction is processed via the oxygen atom.

HOMO/LUMO and MESP for CNT-metal oxides as a complex
HOMO/LUMO orbitals and MESP calculations revealed an observed difference between the two mechanisms of interaction between CNT and metal oxides when the interaction is complex. Figure 10a Fig. 11d-f showed the MESPs for complexed CNT interacted with the three metal oxides under study through the oxygen atom. Similarly, for the complex interactions processed through the oxygen atom, the red color is distributed equally within the models representing CNT-O-Zn, CNT-O-Cu, and CNT-O-Co. As presented in Figs. 9a-c and 11d-f, it is clear that the electronegativity for the adsorbed interaction processed through oxygen is higher than that for the complex interaction. This means that the reactivity of the oxygenated adsorbed interaction is higher than that of the complexed one.

TDM and energy gap ∆E calculation for CNT-metal oxides as adsorb
The reactive property of CNT structure and the interaction of CNT with metal oxides is determined by the two physical parameters: total dipole moment (TDM) and ∆E value. Where the reactivity increased when the TDM increased, and the ∆E decreased. The

TDM and ∆E calculation for CNT-metal oxides as complex state
For CNT-Metal-O interaction, Table 3  Finally, as shown in Table 4 the interaction of ZnO from oxygen atom as complex differs from the expected result. This is because the ZnO is an n-type semiconductor where the valance band is related to the 2p level in oxygen and the conduction bands come from the 4 s level of zinc atom, electrons move from valance bands to conduction bands leaving holes in the valance band (Li et al. 2020;Harun et al. 2016). Therefore in case of the strong interaction between CNT and ZnO, holes directed to transfer between Oxygen to CNT introduced positive charge transfer around the CNT surface. This charge transfer enhanced the reactivity of the composite surface (Gupta and Saleh 2011;Boscarino et al. 2019).

Conclusion
The interaction between CNT and Zn, CuO, and Co 3 O 4 nanoparticles was subjected to quantum mechanical calculations. HF/STO-3G method is suitable for studying the molecular structure of CNT and the interaction of CNT with ZnO, CuO, and Co 3 O 4 . The TDM value, ∆E, and MEP are studied at the same level of theory. The mechanism of the interaction between CNT and nano metal oxides was studied as a complex state and adsorbed state. The MESP studies showed the distribution of charges and the presence of electrophilic-nucleophilic charges in the interaction between CNT and metal oxides in

Conflict of interest The authors have not disclosed any competing interests.
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons licence, and indicate if changes were made. The images or other third party material in this article are included in the article's Creative Commons licence, unless indicated otherwise in a credit line to the material. If material is not included in the article's Creative Commons licence and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this licence, visit http:// creat iveco mmons. org/ licen ses/ by/4. 0/.